stresses at the interface of micro with nano
Post on 11-Dec-2016
Embed Size (px)
Stresses at the Interface of Micro with NanoNicholas Leventis,*, Sudhir Mulik, Xiaojiang Wang, Amala Dass, Chariklia Sotiriou-Leventis, and
Hongbing LuDepartment of Chemistry, UniVersity of MissourisRolla, Rolla, Missouri 65409, and Department of Mechanical
and Aerospace Engineering, Oklahoma State UniVersity, Stillwater, Oklahoma 74078
Received June 2, 2007; E-mail: email@example.com
Bicontinuous materials consisting of an open interconnectedmacroporous system with mesoporous walls create a wide rangeof possibilities for sorption, catalysis, drug delivery, electrochemicalenergy storage, and separations (filtration, HPLC).1,2 In monoliths,macropores provide low hydraulic resistance, hence easy access tothe bulk by pressure-driven flow, whereas the large mesoporoussurface area is always a very short distance away from everywhereand is accessed quickly by diffusion.3 Here we report that in dryform those materials have innate stresses built in at the interfaceof the two size regimes. Relief and stabilization against collapse ispossible by coating all internal surfaces with polymer.
Materials with ordered hexagonal mesopores can be madethrough a modified sol-gel process that involves a surfactant suchas Pluronic P123 (a PEO20PPO70PEO20 triblock copolymer) as astructure directing agent (template). That is, at the right concentra-tion, Pluronic P123 self-assembles in closely packed hexagonalstacks of cylindrical pillars, and subsequently a sol-gel step addssilica filling the voids around them. Post-gelation removal ofPluronic P123 leaves behind a sol-gel material perforated by ahexagonal arrangement of tubes (SBA-15 type materials).4 Thediameter of the tubes can be increased by using a swelling agentsuch as 1,3,5-trimethylbenzene (TMB),4,5 but if the concentrationof TMB is increased above a certain threshold, the result is amesoporous cellular foam (MCF), namely, a bicontinuous macro-porous system with random mesoporous walls.6 If the concentrationof Pluronic P123 by itself or in combination with TMB is adjustedcarefully, the result is a macroporous silica with walls consistingof regular (organized) mesopores.7 For several applications, wetgels of these materials may need to be dried, and the question iswhether macro- and mesopores shrink the same. If not, stressesare included at the interface of the two fractal levels, causing theinherent structural instability associated with a potential collapseor at the very least a dimensional change of the material upondrying. Addressing this question, however, is not trivial because itrequires stabilization of the internal stresses in order to producedry forms preserving the dimensions of wet gels. In other words,the bicontinuous porous system should become capable of resistingshrinkage during drying. This was accomplished by coating allinternal surfaces with a diisocyanate-derived polymer. As it turnsout, shrinkage is indeed different at the nano and the micro sizeregimes.
For our purposes, bicontinuous macro/mesoporous silica wasprepared by Nakanishis modification of Stuckys method wheremesoporous gels rather than precipitates are obtained by reducingthe volume of the sol.7 Typically, Pluronic P123 (P, 4 g) wasdissolved in 1.0 M aqueous HNO3 (12 g), and TBA (T, 0.4 g) wasadded at room temperature. After stirring for 30 min, samples werecooled to 0 C, TMOS (5.15 g) was added, and stirring continued
for another 30 min. The mixture was poured into molds, whichwere kept at 60 C for gelation (110 min). Samples were aged for5 the gelation time. Following Nakanishis notation,7 the materialis referred to as native MP4-T045. However, preparation of dryself-standing monoliths is not straightforward: Nakanishis pro-cedure that calls for drying at 60 C under ambient pressurefollowed by burning Pluronic P123 off at 600 C led to coarsepowders. Structural collapse, with or without prior removal ofPluronic P123 (vide infra), occurs during drying rather than duringcalcination. Therefore, reasoning that surface tension forces on theskeletal framework by the residing vapor/liquid interface might beresponsible for shrinkage,8 we resorted to an aerogel-like workupstrategy: after the template and swelling agent were removed fromthe wet gels by a Soxhlet extraction (CH3CN), pore filling solventswere exchanged with liquid CO2, which was taken out supercriti-cally. This approach did produce monoliths which, as opposed totypical silica aerogels, still shrink significantly (29%) relative tothe dimensions of their wet gels.
In order to lock the skeletal framework at the wet gel stage,immediately after Soxhlet extraction, wet gels were exposed to analiphatic diisocyanate solution (Desmodur N3200 from Bayer) thatreacts both with the surface -OH groups forming urethane andwith adsorbed water forming amines; in turn, amines react withmore diisocyanate from the pores, yielding tethers of polyurea.9Thus, the bulk density of dry monoliths increases by a factor of2.05, but now they shrink only by 13% relative to the molds versus29% of native samples. The diisocyanate-treated material is referredto as X-MP4-T045 (X for cross-linked). Figure 1 compares nativeand X-monoliths at the two size extremes. The presence of thesmall-angle XRD pattern suggests that the mesoporous systems of
University of MissourisRolla. Oklahoma State University.
Figure 1. Left: Photographs of typical dry native (MP4-T045; Fbulk )0.367 ( 0.003 g cm-3; Fskeletal ) 1.935 ( 0.002 g cm-3) and diisocyanate-treated (X-MP4-T045; Fbulk ) 0.755 ( 0.017 g cm-3; Fskeletal ) 1.279 (0.001 g cm-3) bicontinuous meso/macroporous silica monoliths, made usingPluronic P123 as structure directing agent, 1,3,5-trimethylbenzene asswelling agent, and supercritical fluid removal of pore solvents. Both gelswere prepared using 1.04 cm diameter molds, so size differences reflectdifferent shrinkage upon drying. The diameter of the native samples is 0.743( 0.005 cm and of the X-samples it is 0.909 ( 0.007 cm. Right: PowderXRD patterns of samples as indicated. The X-sample shows a smallerdiffraction angle, indicative of a larger spacing between ordered features.
Published on Web 08/14/2007
10660 9 J. AM. CHEM. SOC. 2007, 129, 10660-10661 10.1021/ja074010c CCC: $37.00 2007 American Chemical Society
the two materials are stereoregular and indicates that the orderedfeatures producing the diffraction pattern are spaced further apartin the X-samples, in agreement with the fact that they shrink less.
SEM in combination with TEM confirms the fractal structureof the MP4-T045 material, which consists of macropores (Figure2, left) surrounded by stereoregular mesoporous walls (Figure 3,left). After treatment with diisocyanate, the macroporous structureappears more open (Figure 2, right) in agreement with the largermonolith size, and it still consists of entangled worm-like objectswhose shape is maintained, but they look thicker, suggesting thatnew material (polymer) has been deposited on the macroporoussurfaces conformally. Indeed, the porosity (calculated from bulkand skeletal density data) has been decreased, but not dra-matically: from 81% empty space before polymer treatment to 50%after. By looking inside the worm-like objects, though, the pictureis quite different. First, in TEM (Figure 3, right), the ordered tubularstructure is barely visible, probably due to lack of Z-attenuationbetween the polymer and silica. Second, the BET surface area hasdecreased dramatically, from 612 m2 g-1 for native samples to 2.96m2 g-1 for X-samples! Either mesopores have collapsed completelyor access to them has been blocked at the mouth of the tubes ormesopores have been filled with polymer. XRD data (Figure 1)show that the tubular structure is still present. If polymer had simplyclogged the entrance of the mesopores, the TEM contrast wouldhave been preserved and the tube structure would still be clearlyvisible in Figure 3, right. All data suggest that the polymer hascompletely filled the mesopores, and the net result is that thecomposite material shrinks much less upon drying.
Now, shrinkage at the macroscopic level is quite different fromshrinkage of the mesopores. This is inferred by comparing the ratioof a macroscopic linear dimension (e.g., the monolith diameter)with the ratio of a nanoscopic linear dimension (e.g., the spacingbetween the tubes in the worm-like objects). Thus, (diameter ofX-MP4-T045)/(diameter of native MP4-T045) ) 1.23 and (unit cellof X-MP4-T045)/(unit cell of MP4-T045) ) 1.63. Since X-samplesclosely resemble the wet gels in size and shape, it is clear thatupon drying the spacing between the tubes, and therefore the sizeof the worm-like objects, has been reduced more than the size ofthe monolith, which in turn reflects the average spacing betweenthe worm-like objects. The reasons might not be difficult toreconcile.
All silica surfaces are terminated with silanols, and practicallyall BET surface area is in the tubes where an interesting situationarises: in the concave mesoporous surfaces, hydroxyls point inward,and owing to the small pore diameter, they are forced close to oneanother where they can interact strongly through hydrogen bond-ing.10 The latter pulls the pore walls together; eventually newSi-O-Si bonds are formed in a process that resembles an extremecase of syneresis (shrinking during aging),7 and the worm-likeobjects contract. In contrast, hydroxyls on top of the worm-likeobjects are about as close as on a flat surface. The fact that theworm-like objects tend to shrink introduces stresses at the interfaceof the two size regimes, pulling the worm-like objects apart, andthe structure is expected to become weaker. The tendency of tubularstereoregular mesopores to constrict upon drying explains also thefact that native MP4-T045 monoliths do shrink significantly despiteuse of supercritical fluid CO2 that eliminates surface tension forces.Being a